Abstract
The effect of surface roughness on the Seebeck coefficient in the sub50nm scale silicon ultra thin films is investigated theoretically using nonequilibrium Green's function formalism. For systematic studies, the surface roughness is modelled by varying thickness periodically with square wave profile characterized by two parameters: amplitude (A_{0}) and wavelength (λ). Since high Seebeck coefficient is obtained if the temperature difference between the ends of device produces higher currents and higher induced voltages, we investigate how the generated current and induced voltage is affected with increasing A_{0 }and λ. The theoretical investigations show that pseudoperiodicity of the device structure gives rise to two effects: firstly the threshold energy at which the transmission of current starts is shifted towards higher energy sides and secondly transmission spectra of current possess pseudobands and pseudogaps. The width of the pseudobands and their occupancies determine the total generated current. It is found that current decreases with increasing A_{0 }but shows a complicated trend with λ. The trends of threshold energy determine the trends of Seebeck voltage with roughness parameters. The increase in threshold energy makes the current flow in higher energy levels. Thus, the Seebeck voltage, i.e. voltage required to nullify this current, increases. Increase in Seebeck voltage results in increase in Seebeck coefficient. We find that threshold energy increases with increasing A_{0 }and frequency (1/λ). Hence, Seebeck voltage and Seebeck coefficient increase vice versa. It is observed that Seebeck coefficient is tuneable with surface roughness parameters.
1. Introduction
It is reported that when the two ends of the thermoelectric material are kept at different temperatures, the voltage is generated [1]. This effect is called as the Seebeck effect. This effect has useful applications as it shows that heat can be converted to electricity and vice versa. In the last few years due to quest for finding, the highly efficient ways to produce and use energy there has been an increased interest in the thermoelectric performance of a device [2]. Moreover, thermoelectric energy conversion paves the way for utilization of waste heat generated in the devices into useful electric power. The extraction of waste heat is an important issue, especially nowadays, when the devices are reaching the sub50nm scale. Thus, intensive research has been reported for the effect of dimensionality on the thermoelectric phenomenon [35]. As the dimensions reduce down to sub50nm scale, the surface roughness plays a crucial role in determining the performance of the device. In this scale, the spatial extent of variations due to roughness is comparable to the device dimensions [6]. Hence, the investigation on the effect of surface roughness is important and crucial [79]. In this article, we have made a systematic study of the surface roughness effects on Seebeck coefficient. The surface roughness has been modelled by varying the thickness of the film periodically with a square wave profile as shown in Figure 1. The roughness is characterized by two parameters: amplitude (A_{0}) and wavelength (λ) of the square wave [10]. These parameters are analogous to the root mean square roughness and the roughness autocorrelation length which are commonly used to determine the surface roughness morphology [11]. We study the effect of roughness with increasing A_{0 }and λ on the Seebeck effect. In other words, we investigate how does the induced voltage, V_{Seebeck}, for a fixed temperature difference between the two ends of a device, is affected due to increasing A_{0 }and λ of the surface roughness of the device. To clearly bring the role of surface roughness the electron transport is considered to be coherent inside the device. The phase coherent transport is possible in the devices with the dimensions in the sub50nm scale [12].
Figure 1. The schematic diagram of simulated 2D Si structure. Length of the channel is L_{c}, average thickness is T_{b }and roughness parameters are: amplitude (A_{0}) & periodicity (λ). The bias is applied to nullify the current due to temperature gradient.
When the two ends of the device are subjected to a temperature difference, initially, there is a net flow of current I_{net }from one end of the device to the other as shown in Figure 2a. This is so because, due to temperature difference, there is a different distribution of electrons in different energy states at the two ends. Hence, the number of electrons moving from the cold end to the hot end in an energy level 'ε' is not the same as that of from hot end to cold end. This results in net flow of electrons in an energy level 'ε'. The total current I_{net }is obtained from adding the contributions from all the energy levels. This net flow of current results in an accumulation of electrons at one end which builds an electric field opposing the incoming electrons as shown in Figure 2b. Further accumulation of charge stops when no more electrons are able to make it due to the building of electric field. The voltage developed due to the electric field is called Seebeck voltage V_{Seebeck}. Seebeck coefficient is obtained by dividing the Seebeck voltage by temperature difference [13]. As shown in Figure 2c, Seebeck voltage can be measured by calculating the amount of voltage required 'V_{applied}' to nullify the current 'I_{net}' due to temperature gradient. In this article, we focus on two important issues: firstly we investigate how does, for the same temperature difference between the two ends, I_{net }changes with A_{0 }and λ. Secondly, it has been observed that for some roughness parameters, though the I_{net }decreases but the voltage applied to nullify it, V_{Seebeck}, increases. We investigate the reasons behind this behaviour.
Figure 2. Electron flow for different configurations of device. (a) Electrons flow from hot end to cold end due to temperature gradient. (b) An induced emf is generated due to temperature gradient. (c) Voltage is applied to nullify the current due to temperature gradient. The voltage at which current becomes zero is called Seebeck voltage.
2. Theory
The expression for the current has been calculated using nonequilibrium Green's function formalism (NEGF) [14]. For the devices in the sub50nm scale quantum effects become important and quantum transport model is required for description of transport phenomenon. In this regards, NEGF formalism, in which quantum effects are inherent, provides an efficient framework to model the electron transport in thermoelectric devices. A brief description is given below and detailed development can be found in [15].
The isolated channel and its energy levels are described by Schrodinger equation using Hamiltonian H, potential U and energy eigenvalues of the electron ε_{α}
But when the channel gets connected to the contacts it becomes an open system and the electrons can come and go out of the channel. To represent such an open system, two extra terms get introduced in the Schrodinger equation. The Schrodinger equation becomes
∑_{1 }and ∑_{2}, called selfenergy, represent the coupling between the channel and the two contacts. ∑'s are a complex quantity. Its imaginary part signifies that the electrons can decay out of the channel.
The real part of ∑'s just lifts up the energy eigenvalues of the channel. The second term that gets introduced in the Schrodinger equation is {S}, it is called the source term and is like an actual source driving the system.
Solution of the Schrodinger equation is given by
where
[G] is called the Green's function of the system. In the energy domain, Green function gives the energy eigenvalues for the eigenstates that are occupied in response to the applied impulse.
A_{1}(E) and A_{2}(E) represent density of states due to coupling of the channel with contacts 1 and 2, respectively. The probability of filling of these states is determined by the Fermi Dirac distribution function, f^{1}(E) and f^{2}(E), of the contacts 1 and 2, which are at temperature T and T+ΔT respectively.
Carrier concentration is given by:
The net inflow of current in channel at contact 1 is the same as the net outflow of current at contact 2. Net current flow in channel at contact 1 is the difference between the inflow and outflow of current at contact 1.
If f^{1}(E) = 1 and f^{2}(E) = 0 then T(E) represents the maximum current flow in the channel. For the electron transport in xdirection with confinement present in zdirection, the expression for I(E), after integrating over the energies along ydirection, becomes
where n_{z }is the subband index.
3. Results and discussion
The information about how does I_{net}, i.e. the current due to the temperature gradient, and, V_{Seebeck}, i.e. the voltage required to nullify it, depend on A_{0 }and λ, is obtained by plotting the current voltage (IV) characteristics for devices with different surface roughness parameters. Figure 3 gives the IV characteristics for (a) different amplitudes: A_{0}'s = 0.1 nm, 0.3 nm and 0.5 nm and λ = 2.5 nm and (b) different wavelengths: λ's = 2.5 nm, 3.3 nm and 5 nm and A_{0 }= 0.5 nm. The plot for smooth surface is given in Figure 3a for comparison. The temperature gradient of ΔT = 20 K is applied across the device. The graphs are obtained for the devices in the sub50nm scale by considering the parameters: length of the channel L_{c }= 10 nm and average thickness T_{b }= 2 nm. As I_{net }is the current generated only due to temperature gradient with V_{applied }= 0, it is given by the intercept with the yaxis. It is observed from Figure 3a, b that I_{net }decreases with increasing A_{0 }but with λ there is no definite trend. V_{Seebeck }is the voltage applied to make the current due to temperature gradient equal to zero and is obtained by the intercept with the xaxis. It is observed from Figure 3a, b that V_{Seebeck }increases with increasing A_{0 }and 1/λ.
Figure 3. Currentvoltage characteristics for the 2D Si structure. L_{c }= 10 nm, T_{b }= 2 nm, transport mass m_{x }= 0.19 m_{0}, quantization mass m_{z }= 0.91 m_{0 }and ΔT = 20 K. For (a) λ = 2.5 nm &A_{0}'s = 0.1 nm, 0.3 nm, 0.5 nm and for (b) A_{0 }= 0.5 nm &λ's = 2.5 nm, 3.3 nm, 5 nm. Also in (a) IV characteristics for smooth surface is shown for comparison.
The above trends of I_{net }and V_{Seebeck }with the roughness A_{0 }and 1/λ can be understood by examining the current flowing through each energy level I(E). As seen from Equation 7, I(E) is given as the product of transmission T(E) and
3.1. Effect of roughness on transmission spectra
Figure 4 gives the plots of T(E) for (a) roughness wavelength: λ's = 2.5 nm, 3.3 nm and 5 nm with A_{0 }= 0.5 nm and (b) roughness amplitude: A_{0}'s = 0.1 nm, 0.3 nm and 0.5 nm with λ = 2.5 nm. The following trends are observed: (i) threshold energy, i.e. the 'onset' energy at which the transmission starts, increases with increasing A_{0 }and 1/λ. (ii) There are regions of psuedobands and pseudogaps. The width of the pseudobands decreases with increasing A_{0 }and λ. Within the pseudobands, there are peaks in transmission at some energy. The phenomenon of increase in threshold energy has also been observed experimentally in quantum wells with thickness < 4 nm [16]. We would like to mention here that it has been observed only for thicknesses below 4 nm because surface roughness effects become prominent for ultra thin films. The criterion for the thickness below which surface roughness effects become prominent is discussed in [16]. So, our discussions can be experimentally validated only for ultra thin films. We will analyse the implications of the above trends on I_{net }and V_{Seebeck }but before that we discuss in brief the presence of the above trends.
Figure 4. Energy resolved transmission spectra at zero applied voltage. For (a) A_{0 }= 0.5 nm &λ's = 2.5 nm, 3.3 nm, 5 nm and for (b) λ = 2.5 nm &A_{0}'s = 0.1 nm, 0.3 nm, 0.5 nm. Temperature gradient ΔT = 20 K for both (a, b).
The increase in threshold energy occurs due to the varying thickness seen by the electron while crossing the channel. The regions of the channel where the thickness is large, the confinement is small and the regions where the thickness is small, the confinement is high as seen from Figure 1. Since the lowest value of ε_{z}, which corresponds to the subband energy, depends on the confinement it alternates with the same periodicity as the thickness as shown in Figure 5. The value of ε_{z}, i.e. subband energy is large for high confinement and vice versa. The subband energy corresponds to the potential energy seen by the electron. The electron crossing the channel experiences this varying potential energy landscape which was not the case when the surface was smooth. As the electron crossing the channel moves from the region of low potential energy to the high potential energy it feels an additional confinement effect which was not present for smooth surface. This additional confinement effect causes the increase in lowest energy which the electron can take. Thus, the threshold energy, which corresponds to the lowest energy eigenvalue, increases. The confinement effect will be more for increasing A_{0 }as the electron while moving from low potential energy to high potential energy region sees higher barrier heights. Thus, the lowest energy eigenvalue, i.e. threshold energy, increases with increasing A_{0}. The increase in threshold energy with increasing 1/λ can be explained on the similar lines. The longer λ with the same A_{0 }corresponds to the wider regions of the low potential energy with the same barrier height. This means the confinement effect reduces with increasing λ. Hence, the threshold energy decreases with increasing λ. In other words threshold energy increases with increasing 1/λ.
Figure 5. Suband energy profile along the length of the device. Roughness amplitude (A_{0}) = 0.5 nm and periodicity (λ) = 2.5 nm. The regions of channel at which confinement is high, subbands energies are high and vice versa.
The presence of pseudobands and pseudogaps, a feature of only rough surfaces, is also due to alternate regions of low and high potential energy seen by the electron while crossing the channel. The energy eigenvalues for an electron in such a periodic potential energy profile are given by Kronig Penny model. The solution of the Schrodinger equation for such a potential energy profile shows the presence of energy bands and energy gaps. The investigations on the bandwidth (BW) of the pseudobands with respect to roughness parameters is important as the width of the pseudoband determines the area under the transmission curve and play an important role in determining the total current I_{net}. It is seen from Figure 4a, b that BW of the pseudobands decreases with increasing A_{0 }and λ. These trends of BW on roughness parameters can be understood by looking, again, at the Kronig Penny model. According to Kronig Penny model, if the barrier heights and widths of the periodic potential profile are high, then the BW's are small. This is so because higher barrier heights and widths give smaller tunnelling probability. As the tunnelling probability becomes smaller the BW reduces. Along the same lines increasing A_{0}, which corresponds to higher barrier heights, and increasing λ, which corresponds to larger barrier widths of the pseudoperiodic potential profile, would give rise to smaller BW's. Thus BW decreases with increasing A_{0 }and λ.
3.2. Effect of roughness on total current I_{net}
As I_{net }represents the current only due to temperature gradient with V_{applied }= 0, it is given by the intercept with the yaxis of IV characteristics. It is observed from Figure 3a that I_{net }decreases with increasing amplitude but Figure 3b shows that there is no definite trend with λ. These features can be explained by considering that total current depends on the bandwidth of the pseudobands and their occupancy. For increasing A_{0 }as seen from Figure 4b, threshold energy increases and BW of the pseudobands decreases. The smaller bandwidths along with their presence at higher energy sides result in the decrease in occupancy of these bands. This, in turn, decreases the total no. of carriers contributing to the current. Thus, I_{net }decreases with increasing A_{0}. The trends of I_{net }with λ are complicated. As seen from Figure 4a though the pseudobands are present at lower energy sides with increasing λ but their BW decreases. Thus, on one hand their presence at lower energy sides increases the occupancy on the other hand smaller bandwidths decrease the total occupancy which is obtained by summing the occupancy from all energy levels. These two competing features complicate the trends of I_{net }with λ. Figure 4a shows that BW for λ = 3.3 nm is smaller than λ = 2.5 nm but since the band is present at lower energy sides its occupancy is more. This results in more current for λ = 3.3 nm than for λ = 2.5 nm. For λ = 5 nm the BW is so small that the current is the least.
3.3. Effect of roughness on Seebeck voltage V_{Seebeck }and Seebeck coefficient
As already mentioned V_{Seebeck }increases with increasing A_{0 }and 1/λ. This trend can be understood by examining the circumstances for which I_{total }(= I_{net}) becomes zero. I_{total }is the sum of current from all energy levels, i.e. I = ∫I(E)dE. Figure 6c gives I(E) versus E for λ = 2.5 nm and A_{0 }= 0.5 nm. It is seen that below E_{null }the current is +ve and above E_{null }the current is ve. Hence, the total current obtained by the sum of current from all
energy levels is small. We need to check when does it become zero. As seen from Equation
(7), I(E) is product of transmission T(E) and
Figure 6. Energy resolved transmission, Fermi Dirac occupancy and current for λ = 2.5 nm and 3.3 nm with A_{0 }= 0.5 nm. Energy resolved transmission is shown in (a, d), difference in the Fermi Dirac occupancy of cold and hot ends is shown in (b, e) and current is shown in (c, f). For (ac) λ = 2.5 nm and for (df) λ = 3.3 nm. E_{null }shifts towards higher energy sides with decreasing wavelength.
To understand how does E_{null }shifts towards higher energy states with increasing V_{applied}, we observe that as the threshold energy increases the electrons occupy higher energy
states and the current contributions come from higher energy levels. The net current
I_{net}, which flows from hot side to cold side is also made of electrons flowing in higher
energy levels. We need to apply voltage, V_{Seebeck}, to nullify this current I_{net}. Thus, we need to increase the potential of the cold side so that electrons at the
cold side occupy higher energy states to balance this current. Thus, as the threshold
energy increases we need to apply higher V_{Seebeck }to balance the net current. Also, since the occupancy of higher energy states at the
cold side increases with increasing V_{Seebeck }the E_{null}, for which
Table 1. Variation of Seebeck coefficient for different roughness amplitudes
Table 2. Variation of Seebeck coefficient for different roughness wavelengths
For the devices if A_{0 }is increased at constant λ it is observed that though I_{net }decreases but still V_{Seebeck }increases. This happens because BW decreases and threshold energy increases. Smaller BW's at higher energy sides reduce occupancy and hence I_{net}. Though the current reduces, it is made up of electrons present in higher energy levels and as already explained higher voltages are required to nullify the current from higher energy states.
The discussions show that it is the increase in threshold energy which causes the current to flow in the higher energy levels and hence results in increase in Seebeck coefficient. This result implies that any physical geometry whether periodic or aperiodic which results in an increase in threshold energy will show an increase in Seebeck coefficient. It also implies that if the threshold energy dependence on roughness parameters become feeble then Seebeck coefficient will saturate, i.e. it will not change much with the change in roughness parameters. The detailed investigations on the above two implications are in progress.
4. Conclusions
The surface roughness causes the net current I_{net}, produced due to the temperature gradient, to decrease with increasing roughness A_{0 }but trends with λ are complicated. The voltage V_{Seebeck}, required to nullify this I_{net }shows a definite trend. It increases with increasing A_{0 }and 1/λ. Increase in V_{Seebeck }results in increase in Seebeck coefficient. The reasons for the above trends have been attributed to the varying periodic thickness seen by the electron crossing the channel. The periodically varying thickness corresponds to varying confinement and hence periodically varying subband energy. The subband energy corresponds to the potential energy seen by the electron. For the electron moving in a pseudoperiodic potential, the transmission spectra shows the following features: (1) The threshold energy at which the transmission of current starts is shifted towards higher energy sides. It increases with increasing A_{0 }and 1/λ. (2) There are regions of pseudobands and pseudogaps. The BW of the pseudobands decreases with increasing A_{0 }and λ.
The above features of transmission spectra result in following trends for I_{net }and V_{Seebeck}: (1) It is observed that BW decreases and shift towards the higher energy sides for increasing A_{0}. Both these features result in reduced occupancy of the band and hence total carrier concentration. Since I_{net }depends on the total carrier concentration thus I_{net }reduces with increasing A_{0}. (2) It is observed that pseudobands are present at lower energy sides with increasing λ but their BW decreases. Thus, on one hand the presence of bands on the lower energy side increases the occupancy and on the other hand the smaller bandwidth reduces the total occupancy. These two competing features give rise to complicated trends of I_{net }with λ. (3) The trends of threshold energy determine the trends of V_{Seebeck }with roughness parameters. The increase in threshold energy results in the electrons to occupy higher energy states. Thus the net current I_{net }flowing from hot to cold end is made up from higher energy levels. To nullify this current, the occupancy of higher energy states at the cold end is increased by applying higher voltages. Thus higher threshold energy requires higher applied voltages, V_{Seebeck}, to nullify the current. Since threshold energy increases with increasing A_{0 }and 1/λ, hence V_{Seebeck }and Seebeck coefficient increases vice versa. (4) The dependence of Seebeck coefficient on roughness parameters suggest that it can be tailored by choosing the appropriate roughness parameters.
Competing interests
The authors declare that they have no competing interests.
Authors' contributions
MK carried out the NEGF calculations and implemented the code. AB and SN conceived of the study. AB participated in the NEGF calculations and implementation of the code. SN, with the perspective of designing the device in his lab, participated in the discussions of theoretical results and provided the information of the related experimental works. All authors read and approved the final manuscript.
Acknowledgements
SN acknowledges the financial support from Department of Atomic Energy, BRNS, Mumbai, India (grant no.2010/34/47/BRNS/2317). MK thanks Prof. Arun Kumar (IIT Delhi) for help and support during the preparation of manuscript.
References

Jang M, Park Y, Jun M: The characteristics of Seebeck coefficient in silicon nanowires manufactured by CMOS compatible process.
Nanoscale Res Lett 2010, 5:16541657. PubMed Abstract  Publisher Full Text  PubMed Central Full Text

Shakouri A: Recent development in semiconductor thermoelectric physics and materials.
Annu Rev Mater Res 2011, 41:399431. Publisher Full Text

Hicks LD, Dresselhaus MS: Effect of quantumwell structure on thermoelectric figure of merit.
Phys Rev B 1993, 47:1272712731. Publisher Full Text

Kim R, Datta S, Lundstorm MS: Influence of dimensionality on thermoelectric device performance.
J Appl Phys 2009, 105:034506034511. Publisher Full Text

Demchenko DO, Heinz PD, Lee B: Determining factors of thermoelectric properties of semiconductor nanowires.
Nanoscale Res Lett 2011, 6:502. PubMed Abstract  BioMed Central Full Text  PubMed Central Full Text

Andrei P, Mayergoyz I: Quantum mechanical effects on random oxide thickness and random doping induced fluctuations in ultrasmall semiconductor devices.
J Appl Phys 2003, 94:71637172. Publisher Full Text

Markussen T, Jauho AP, Brandbyge M: Surface decorated silicon nanowires: a route to highZT thermoelectrics.
Phys Rev Lett 2009, 103:055502055505. PubMed Abstract  Publisher Full Text

Hochbaum AI, Chen RK, Delgado RD, Liang WJ, Garnett EC, Najarian M, Majumdar A, Yang PD: Enhanced thermoelectric performance of rough silicon nanowires.
Nature 2008, 451:163168. PubMed Abstract  Publisher Full Text

Zianni X: Efficient thermoelectric energy conversion on quasilocalized electron states in diameter modulated nanowires.
Nanoscale Res Lett 2011, 6:286. PubMed Abstract  BioMed Central Full Text  PubMed Central Full Text

Low T, Ansari D: Signature of quantum transport through two dimensional structures with correlated and anticorrelated interfaces.

Goodnick SM, Ferry DK, Wilmsen CW, Liliental Z, Fathy D, Krivanek OL: Surface roughness at the Si(100)SiO_{2 }interface.
Phys Rev B 1985, 32:81718186. Publisher Full Text

Schliemann A, Worschech L, Forchel A, Curatola G, Iannaccone G: Universal signature of ballistic transport in nanoscale field effect transistors.

Bulusu A, Walker DG: Quantum modelling of thermoelectric properties of Si/Ge/Si superlattices.

Wu Y, Childs PA: Conductance of Graphene nanoribbon junctions and the tight binding model.

Datta S: Quantum Transport: Atom to Transistor. New York: Cambridge University Press; 2005.

Uchida K, Watanabe H, Kinoshita A, Koga J, Numata T, Takagi SI: Experimental study on carrier transport mechanism in ultrathinbody SOI n and pMOSFETs with SOI thickness less than 5 nm.